# Investigation of interactions in two-dimensional electron ... · Investigation of interactions in...

date post

17-Aug-2019Category

## Documents

view

213download

0

Embed Size (px)

### Transcript of Investigation of interactions in two-dimensional electron ... · Investigation of interactions in...

Investigation of interactions

in two-dimensional electron gases

with angular resolved photoemission spectroscopy

Carola Straÿer

PhD Thesis

Max Planck Institute for Solid State Research in Stuttgart

Ecole Polytechnique Fédérale de Lausanne

March 25, 2015

ii

Abstract

In this thesis, angular resolved photoemission spectroscopy (ARPES) is used to study

the electronic structure of di�erent two-dimensional electron systems (2DES). This tech-

nique is very surface sensitive and the most direct method to probe the surface band

structure of a system. In addition to the band dispersion also signatures from interac-

tions can be detected with ARPES. A careful analysis of peak position and linewidth gives

access to the complex self-energy Σ, which describes the energy renormalization and the

lifetime of the electrons due to many-body interactions. By using circularly polarized light

it is possible to excite electrons selectively and to extract additional information about the

electronic states in the surface.

2DESs exist typically either at interfaces or at surfaces. We put our focus on the

surface states of topological insulators and investigate Bi2Te2Se and TiTe1.5Se0.5. The �rst

is known to be a topological insulator with the Fermi energy located in the bulk band gap.

A time-dependent doping behavior is observed and we show that the Coulomb interaction

in this material is strongly dependent on the charge carrier density and not negligible for

very low concentrations. TiTe1.5Se0.5 was predicted to be a topological insulator. We are

able to present the surface band structure, but due to the fact that ARPES can only probe

the occupied states it is impossible to see the predicted topological surface states.

The third system under investigation is a monolayer of epitaxial graphene on SiC(0001)

decorated by small amounts of Tl adatoms. ARPES measurements at very low temperature

and very low impurity concentrations show that Tl adatoms not only give rise to electron

doping but have also a large e�ect on the quasiparticle scattering rate. The adatoms

introduce disorder and act on the graphene electronic structure both as Coulomb long-

range scatterers as well as short-range scatterers with a δ-like potential. We show that

also for charged impurities short-range scattering can play an important role and is not

always negligible. By modeling the self-energy for long- and short-range scattering, we

are able to extract a strong short-range scattering potential δ = −3.2 ± 1 eV. A detailedunderstanding of the underlying scattering mechanisms in graphene is very important for

the development of novel impurity-graphene-based electronics.

ARPES experiments are also performed on the surface alloys on Ag(111). For these

measurements, we use circularly polarized light and take advantage of the fact that the

interaction between light and matter changes for di�erent polarizations. Surface alloys on

Ag(111) are formed by depositing 1/3 of a monolayer of bismuth or antimony on the clean

Ag(111) surface, where every third Ag atom is replaced by such an alloy atom. These sys-

iii

tems are known for their Rashba type spin splitting and the resulting chiral spin structure

in the two-dimensional (2D) band structure. We show that circular dichroism (CD) in the

angular distribution of the photoelectrons depends strongly on the experimental setup and

the energy of the photons. Only under special circumstances it is possible to use CD to

access the orbital angular momentum and � in systems with high spin-orbit coupling �

maybe even the spin texture of the surface. Because of the �nal state e�ects, interpretation

of CD data is quite complicated and has to be done very cautiously.

Keywords: ARPEStwo-dimensional electron systemsgraphenetopological insulatorsurface alloysscattering mechanismsCoulomb interactionorbital angular momentumspintronics

iv

Zusammenfassung

In der vorliegenden Arbeit wird die elektronische Struktur von verschiedenen zwei-

dimensionalen (2D) Elektronensystemen mit winkelaufgelöster Photoemission untersucht.

Diese Technik ist sehr ober�ächensensitiv und ermöglicht es direkt die Ober�ächenband-

struktur eines Materials zu messen. Nicht nur die Dispersion der Bänder sondern auch

elektronische Wechselwirkungen können gemessen werden. Durch sorgfältige Bestimmung

von Peakpositionen und -breiten kann man die komplexe Selbstenergie Σ berechnen, die den

Ein�uss der Wechselwirkung von Elektronen mit anderen Teilchen auf die Bindungsener-

gie und die Lebensdauer der Elektronen beschreibt. Wählt man die zirkular polarisiertes

Licht, ist es sogar möglich gezielt Elektronen anzuregen und zusätzliche Information über

die elektronischen Zustände an der Ober�äche zu gewinnen.

2D Elektronensysteme existieren typischerweise entweder an Grenz�ächen oder an Ober-

�ächen. Wir legen unseren Fokus auf die Ober�ächenzustände von topologischen Isolatoren

und untersuchen Bi2Te2Se und TiTe1.5Se0.5. Das erste Material ist bekannt als toloplogi-

scher Isolator, bei dem die Fermienergie in der Bulkenergielücke liegt. Wir beobachten ein

zeitabhängiges Dopingverhalten und wir können zeigen, dass die Coulomb-Wechselwirkung

in diesem Material stark von der Ladungsträgerdichte abhängt und für kleine Ladungsträ-

gerdichten nicht vernachlässigbar ist. TiTe1.5Se0.5 wurde als neuer topologischer Isolator

vorgeschlagen. Wir präsentieren die Ober�ächenbandstruktur, allerdings ist es nicht mög-

lich die topologischen Ober�ächenzustände zu beobachten, da mit Photoemission unbe-

setzte Elektronenzustände nicht gemessen werden können.

Das dritte System, das wir im Folgenden untersuchen werden, ist eine Monolage von

epitaktischem Graphen auf SiC(0001) bedeckt mit einer kleinen Menge von Thalliumada-

tomen. Photoemissionsmessungen bei sehr tiefen Temperaturen und sehr kleinen Konzen-

trationen zeigen, dass Thalliumatome nicht nur Elektronen abgeben sondern auch einen

groÿen Ein�uss auf die Streurate der Elektronen haben. Die Adatome bringen Unordnung in

das System und wirken auf die elektronischen Struktur von Graphen sowohl als Coulomb-

Streuer als auch als kurzreichweitige Streuzentren mit einem δ-förmigen Streupotential.

Wir zeigen, dass auch für geladene Streuzentren kurzreichweitige Streumechanismen eine

wichtige Rolle spielen können und nicht immer vernachlässigbar sind. Durch Modellie-

rung der Selbstenergie für lang- und kurzreichweitige Streuung sind wir in der Lage für

das δ-Potential einen Wert von δ = −3.2 ± 1 eV zu extrahieren. Die zugrunde liegendenStreumechanismen in Graphen zu verstehen ist ein sehr wichtiges Ziel im Hinblick auf die

Entwicklung von elektronischen Bauteilen, die auf mit Störstellen dekoriertem Graphen

v

basieren.

Auÿerdem zeigen wir Ergebnisse von Experimenten an Ober�ächenlegierungen auf

Ag(111). Für diese Messungen verwenden wir zirkular polarisiertes Licht und nutzen den

Vorteil, dass sich die Wechselwirkung zwischen Licht und Materie für verschiedene Polari-

sationen ändert. Ober�ächenlegierungen auf Ag(111) bilden sich, wenn man 1/3 Monolage

Wismuth oder Antimon auf eine saubere Silberober�äche aufdampft. Dabei wird jedes drit-

te Silberatom von einem solchen Legierungsatom ersetzt. Diese Legierungen sind bekannt

für die Rashba-artige Spinaufspaltung und die daraus resultierende chirale Spin-Struktur

in der 2D Bandstruktur. Wir zeigen, dass zirkularer Dichroismus in der Winkelvertei-

lung der Photoelektronen stark von der Geometrie des Experiments und der Energie der

Photonen abhängt. Nur unter speziellen Umständen ist es möglich zirkularen Dichoris-

mus zu benutzen um experimentellen Zugang zum Bahndrehmoment und � in Systemen

mit hoher Spin-Bahn-Wechselwirkung � vielleicht sogar zur Spintextur der Ober�äche zu

bekommen. Aufgrund des starken Ein�usses der Endzustände ist die Interpretation von

Dichroismusdaten höchst komplex und muss besonders vorsichtig durchgeführt werden.

Stichwörter: winkelaufgelöste Photoemissionzweidimensionale ElektronensystemeGraphenTopologischer IsolatorOber�ächenlegierungenStreuungsmechanismenCoulomb WechselwirkungBahndrehmomentSpintronik

vi

Contents

1 Introduction 1

2 Scienti�c Background 5

2.1 Electrons in low dimensions . . . . . . . . . . . . . . . . . . . . . . . . . . 5

2.1.1 Electrons in solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6

2.1.2 Surface states . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7

2.2 Spin-polarized surface states . . . . . . . . . . . . . . . . . . . . . . . . . . 8

2.2.1 The Rashba e�ect . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9

2.2.2 Topological insulators . . . . . . . . . . . . . . . . . . . . . . . . . 11

2.3 Surface states vs. 2D states . . . . . . . . . . . . . . . . . . . . . . . . . . 13

2.3.1 Surface alloys . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 14

2.3.2 Graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15

3 Experimental Techniques 19

3.1 Photoemission spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . 19

3.1.1 The photoemission process . . . . . . . . . . . . . . . . . . . . . . . 19

3.1.2 Quasiparticle picture . . . . . . . . . . . . . . . . . . . . . . . . . . 23

3.2 Angular resolved photoemission . . . . . . . . . . . . . . . . . . . . . . . . 25

3.3 Core level spectroscopy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 29

4 Coulomb interaction in topological insulators 31

4.1 Bi2Se3, Bi2Te3 and Bi2Te2Se . . . . . . . . . . . . . . . . . . . . . . . . . . 32

4.2 Doping behavior . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33

4.3 Coulomb interaction at low charge carrier densities . . . . . . . . . . . . . 34

4.4 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 38

vii

Contents

5 Surface band structure of TiTe1.5Se0.5 43

5.1 Search for new topological materials . . . . . . . . . . . . . . . . . . . . . . 43

5.2 Crystal structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 44

5.3 Electronic structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 45

5.4 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 48

6 Scattering mechanisms in thallium doped epitaxial graphene 51

6.1 Impurities on graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 52

6.2 Doping e�ect of Tl adatoms . . . . . . . . . . . . . . . . . . . . . . . . . . 53

6.3 Linewidth analysis and theoretical description . . . . . . . . . . . . . . . . 56

6.3.1 Long-range scattering . . . . . . . . . . . . . . . . . . . . . . . . . . 56

6.3.2 Short-range scattering . . . . . . . . . . . . . . . . . . . . . . . . . 58

6.4 Graphene as topological insulator . . . . . . . . . . . . . . . . . . . . . . . 59

6.5 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 61

7 Circular dichroism in the band structure of surface alloys 63

7.1 Circular dichroism in the angular distribution of photoelectrons . . . . . . 64

7.2 Photoemission experiments . . . . . . . . . . . . . . . . . . . . . . . . . . . 65

7.3 Theoretical description . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67

7.4 Orbital angular momentum in surface alloys . . . . . . . . . . . . . . . . . 69

7.5 Photon-energy dependence . . . . . . . . . . . . . . . . . . . . . . . . . . . 70

7.6 Discussion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 72

8 Summary and Outlook 75

8.1 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 75

8.2 Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 76

8.2.1 Topological insulators . . . . . . . . . . . . . . . . . . . . . . . . . 77

8.2.2 Circular dichorism measurements . . . . . . . . . . . . . . . . . . . 78

8.2.3 Graphene . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 78

viii

Chapter 1

Introduction

�God made the bulk; surfaces were invented by the devil.� [1] As the quote from Wolfgang

Pauli hypothesizes, the physics of surfaces is quite di�erent compared to the bulk. One

reason for the di�erent behavior is the dimensional constraints of the electrons. Since the

beginning of the 20th century it is known that in low-dimensional materials the limits of

classical physics are reached. As soon as the dimensions of an object are smaller than

the wavelength of the conduction electrons, quantum phenomena emerge. Surfaces can be

described as two-dimensional electron systems (2DESs) where the electrons are con�ned in

one direction but can move freely in the plane. Some famous examples for physical e�ects

that can only be explained by a quantum-mechanical picture like the quantum Hall e�ect

are found in 2DES [2�4].

For investigation of such phenomena, accurate fabrication of low-dimensional materials

is required. The enormous development of technical knowledge and experimental methods

in the last decades allows scientists to design and investigate new low-dimensional systems

with fascinating properties that can be described by quantum mechanics. It is possible

to study materials at the nanoscale in real space with atomic force microscopy (AFM)

and scanning tunneling microscopy (STM). For determination of the atomic structure at

the surface low energy electron di�raction is a very useful technique. To explore the

electronic structure at the surface x-ray photoelectron spectroscopy (XPS) and angular

resolved photoemission spectroscopy (ARPES) are the methods of choice. In this thesis,

the electronic properties of 2DESs localized at the surface are investigated using ARPES.

In particular, the focus of this thesis lies on topological insulators (TIs). TIs are

materials that have an insulating bulk but are conducting on their surface. The conduct-

ing surface states are very interesting due to their spin polarization and their robustness

1

Chapter 1. Introduction

against defects. Many of them have a linear dispersion relation and are very promising

candidates for fast spintronic devices. Common theoretical descriptions of TIs are for-

mulated in terms of single-particle quantum mechanics [5]. Usually, the electron-electron

interaction is neglected since the dielectric constant in TIs is extremely high and the inter-

action is e�ectively screened. However, the strength of the interaction is also dependent

on the charge carrier density. If the charge carrier density is low enough, electron-electron

interaction can play an important role - it can even turn the topological phase into an insu-

lating ground state [6]. Therefore, it is a crucial issue to understand the interplay between

strong electron-electron interactions and the topological surface states. While studying

the Coulomb interaction in Bi2Te2Se it was found that the bands are substantially a�ected

by the electron-electron interaction. Depending on the charge carrier density the band

structure is renormalized and in addition an aging-induced band bending was observed.

Beside the detailed investigation of known TIs, it is also very important to look for new

topological materials. In this thesis �rst results of an ARPES study of TiTe1.5Se0.5, which

is assumed to be a TI, are presented. Due to their high atomic spin-orbit coupling (SOC)

strength transition metal dichalcogenides are very promising candidates for materials with

a topologically nontrivial surface state. Some theoretical studies predicted TiS2−2xTe2xto turn into a TI for 0.48 < x < 0.80. To check if TiTe1.5Se0.5 behaves similarly the

�rst ARPES measurements on this system were performed. The band structure looks

promising, but to identify the systems as a TI, further studies are necessary since the

assumed topological surface states are located in the unoccupied states.

In addition to TIs, epitaxial graphene on SiC(0001) was studied. It was shown that

chemical doping is an e�cient method to tune the electronic structure and to shift the

Fermi level in either direction. However, every time dopants are deposited on graphene they

unavoidably introduce disorder and change the charge carrier mobility. A very important

issue for the development of future electronic devices based on impurities on graphene is the

ability to predict the involved scattering mechanisms and account for them accordingly. In

general, long-range scattering is said to be the dominant scattering mechanism in graphene

transport devices. For thallium atoms on graphene, which can be considered paradigm

long-range scatterers, signi�cant scattering contributions from short-range scattering were

found. Using signatures of quasiparticle scattering in the photoemission spectral function

and a self-energy model for both long-range and short-range scattering mechanisms, Tl

adatoms could be identi�ed also as e�cient short-range scattering centers.

In the third topic of this thesis, the use of circular dichroism (CD) measurements as

2

a method to access the orbital angular momentum (OAM) or even the spin of a surface

state is discussed. Surface alloys on the Ag(111) surface show a large spin splitting in

the surface states due to the Rashba-Bychkov e�ect [7]. Besides the great potential for

applications in the �eld of spintronics, these alloys are also perfect test systems for surfaces

with giant spin splitting. By using circularly polarized light one can measure a CD signal

in the surface alloys on Ag(111). It was found that the CD signal is strongly dependent

on the photon-energy and does not directly contain information about the spin. Instead of

following the spin direction, CD is dominated by the geometry of the experimental setup,

by the dipole selection rules and by the �nal state.

This thesis is organized as follows: In Chap. 2 an introduction to the scienti�c back-

ground required for the understanding of the experimental results is given. Chap. 3 de-

scribes the technical background and the experimental setups that were used to carry out

the experiments. The results from the studies about the electron-electron interaction in

TIs are presented in Chap. 4. In Chap. 5 the surface band structure of a titanium dichalo-

genide is introduced. Chap. 6 is dedicated to our experimental results on Tl doped epitaxial

graphene. In Chap. 7 the possibility of accessing the spin orientation in surface states using

circularly polarized light in ARPES experiments is discussed. Finally, a detailed summary

of the main results is given in Chap. 8 and some ideas for future research projects based

on the previous chapters will be presented.

3

Chapter 1. Introduction

4

Chapter 2

Scienti�c Background

In solid state physics the main focus is on crystals and the investigation of their properties.

Scientists are interested in electrical, magnetic, optical, or mechanical characteristics. In

addition to the crystal structure, the electronic properties of a solid are of special interest.

The latter are determined by the electrons inside the crystal. Moreover the potential in

which the electrons are embedded plays a very important role. For example, electrons in

a low-dimensional environment behave quite di�erent from free electrons.

2.1 Electrons in low dimensions

Generally, electrons in solids move in three dimensions, but by reducing the spatial char-

acteristics of the crystal, for example, by creating surfaces or interfaces, electrons can be

forced to stay in less than three dimensions. If they are con�ned to certain directions or

planes, their energy E and momentum ~k in the relevant direction will be quantized. In

a quantum well, electrons are con�ned in only one direction, in a quantum wire they are

con�ned in two directions and in a quantum dot con�nement exists in all three directions.

The simplest case of electron con�nement is shown by an electron in a potential well

in one dimension. The potential well of the length L is shown in Fig. 2.1 (a) and can be

described by [8, 9]

V (x) =

0, for 0 < x < L∞, elseSolving Schrödinger's equation for this potential gives the same dispersion relation as

5

Chapter 2. Scienti�c Background

E

x0 L

V(x)=∞ V(x)=∞

V(x)=0

barrier well barrier

(a) (b)

k

E4

E3

E2

E1

k1 k2 k3 k4

Figure 2.1: One-dimensional quantum well: (a) Outside the one-dimensional well the bar-riers have in�nitely large potential, while inside the potential is zero. (b) The energy of anelectron in a one-dimensional quantum well (black circles) and a free electron (red line), bothdepend on the wave vector in the same way [see Eq. 2.1]. However, the electron in the wellmay only have certain, discrete energy levels.

for free electrons

E(~k) =~2~k2

2m(2.1)

but for the potential well there are only discrete momentum values allowed that satisfy

k = nπ/L with n ∈ N [see Fig. 2.1 (b)]. ~ represents Planck's constant h divided by 2πand m is the mass of the electron.

Con�ned electron systems are of particular interest because they give access to special

physical phenomena that are based on quantum physics. Particularly, in two dimensions i.e.

at surfaces or interfaces, many interesting physical e�ects can happen, like the (fractional)

quantum Hall e�ect [10]. In this thesis we are focusing on electrons at surfaces, i.e. on

2DES.

2.1.1 Electrons in solids

In a very simple picture solids can be modeled by atoms of the same kind that come close

together. Electrons in solids feel a periodic potential V (~r) = V (~r + ~R) where ~R gives the

lattice periodicity [8]. The solutions for the Schrödinger equation with such a potential

are Bloch waves Ψk(~r) = uk(~r)ei~k~r with uk(~r) = uk(~r + ~R). Accordingly, also the energy

eigenstates show periodic behavior and the free electron parabola is duplicated at every

lattice vector, as shown schematically in Fig. 2.2 (a) and (b).

Since the band structure is periodic in ~R it is su�cient to draw the bands only in the

6

2.1. Electrons in low dimensions

Momentum

Ene

rgy

Momentum

(a) (b) (c)

-π/a π/a

Momentum

-π/a π/a-2π/a 2π/a0

Figure 2.2: Electronic band structure for electrons in a periodic potential: (a) The freeelectron parabola. (b) Periodic zone scheme of the band structure in a solid. (c) Reducedzone scheme in the �rst Brillouin zone.

�rst Brillouin zone like in Fig. 2.2 (c). Due to the lattice potential small energy gaps will

be opened at the crossing points which lead to the electronic band structure that consists

of the allowed bands and band gaps [not shown in Fig. 2.2].

2.1.2 Surface states

As shown in Sec. 2.1.1 the solutions to the Schrödinger equation in an in�nite crystal are

Bloch waves. By creating a surface the potential deviates from its perfect periodicity. For

a potential that is not perfectly periodic there are additional solutions for the Schrödinger

equation that can be divided into two groups: (i) the Bloch waves, which decay expo-

nentially into vacuum [see Fig. 2.3 (a)] and (ii) states, which are damped exponentially

into the vacuum as well as into the bulk. The latter are the so-called surface states and

are schematically drawn in Fig. 2.3 (b). Their energy eigenvalues are located in the pro-

jected bulk band gap and their wave vector k|| is imaginary. Electrons within these surface

states are strongly con�ned in the direction perpendicular to the surface, whereas they can

propagate freely within the surface. Therefore, surface states constitute a 2DES.

In the discussion of surface states one distinguishes Shockley states from Tamm states

[11]. In principle both are terms for the description of the same physical phenomenon,

i. e. surface states but the mathematical approach is di�erent. Shockley surface states are

described in the framework of the nearly free electron model for clean and ideal surfaces and

exist simply due to crystal termination at the surface [12]. In contrast, the Tamm states

7

Chapter 2. Scienti�c Background

bulk vacuum

bulk state

bulk vacuum

surface state(a) (b)

Figure 2.3: (a) In a semi-in�nite crystal the Bloch waves are exponentially damped in thevacuum region. (b) Due to the missing periodicity at the surface there are additional solutionsto the Schrödinger equation, which have imaginary wave vector. They decay exponentiallyinto vacuum as well as into the bulk.

are obtained using the tight binding model. The existence of Tamm surface states implies a

considerable perturbation of the potential in the surface region due to reconstruction [13].

In addition to these surface states, there are surface resonances that decay exponentially

into vacuum but show a sizable amplitude in the bulk.

2.2 Spin-polarized surface states

In general, in a three-dimensional (3D) solid time reversal [E(↑, ~k) = E(↓,−~k)] as wellas spatial inversion symmetry [E(↑, ~k) = E(↑,−~k)] are ful�lled. The combination of bothgives rise to Kramers spin degeneracy [14], expressed as

E(↑, ~k) = E(↓, ~k)

However, SOC can lift the spin degeneracy if one of the symmetries is broken [15].

In current surface science research, there are two main classes of spin-polarized surface

states [16,17] that are of interest; Rashba-split surface states and the surface states in TIs.

In the next two sections both will be introduced and compared to each other.

8

2.2. Spin-polarized surface states

2.2.1 The Rashba e�ect

The spatial inversion symmetry of a solid can be easily broken, for example, due to bulk

inversion asymmetry in noncentrosymmetric semiconductors. As a consequence of SOC the

spin degeneracy can be removed [18�20]. Also, a structural inversion asymmetry, which is

caused simply by the presence of the surface in a semi-in�nite crystal, breaks space inversion

symmetry. Electronic states at the surface feel the structural inversion asymmetry and

become spin-polarized due to SOC. The case in two dimensions (2D) is usually considered

as the Rashba-e�ect [7,21]. For the theoretical description of the spin splitting in a 2DES

with inversion asymmetry along the z-direction, the Rashba Hamiltonian is added to the

quasi-free 2D electron gas con�ned in the (x; y)-plane. The Hamiltonian describes SOC in

propagating electronic states and is given by

HRB = αR~σ(~k|| × ~ez) (2.2)

with the Rashba parameter αR determined by the potential gradient perpendicular to the

2DES, the Pauli matrices ~σ = (σx, σy, σz), the electron momentum in the plane ~k|| and the

unit vector ~ez perpendicular to the plane of the 2DES. Solving the Schrödinger equation

for the Rashba Hamiltonian gives

E(k||) = E0 +~2k2||2m∗

± αRk|| = E0 +~2

2m∗(k|| ± kR

)2for the energy dispersion. The resulting band structure consists of two parabolas with

an e�ective mass m∗, which are shifted by the momentum o�set ±kR = αRm∗/~2 fromthe original momentum. However, at high symmetry points the dispersion has to be spin

degenerate because of time reversal symmetry. A typical dispersion is schematically drawn

in Fig. 2.4 (a) and (b).

A third characteristic parameter that results from the momentum o�set kR is the so

called Rashba energy ER = ~2k2R/(2m∗) = m∗α2R/(2~2). It describes the energy di�erencebetween the band extremum and the crossing point at the high symmetry point. A cut

through the band structure at a constant energy above the crossing point gives two concen-

tric circles [see Fig. 2.4(c)]. Due to the vector product in Eq. 2.2 the spin vector is expected

to be entirely in-plane, i.e. perpendicular to ~ez and perpendicular to the momentum k||of the electron. Consequently the spin vector points tangential along the constant energy

contours; it rotates clockwise on the inner circle and counterclockwise on the outer one.

9

Chapter 2. Scienti�c Background

Wave Vector k||

ER

kRαR>0

Initi

al S

tate

Ene

rgy

E

Wave Vector k||

αR=0(a) (b) (c)

Figure 2.4: Energy dispersion of a 2D electron gas (a) without and (b) with Rashba SOC.The characteristic parameters of the model, ER and kR, are marked. (c) Spin polarisation ona constant energy contour above the crossing point.

However, in total the system is not magnetic since an integration over the whole reciprocal

space gives no net spin.

The �rst example for a Rashba-split surface state is the one on Au(111). LaShell et

al. [22] observed an energy splitting that is proportional to the wave vector and about

110meV at the Fermi level. Di�erent approaches have been chosen to tune [23] or to

enhance the spin splitting for example by adsorption of Ar, Kr or Xe [24].

In order to be able to manipulate the spin splitting at the surface in a desired fashion,

it is very important to understand the underlying mechanism. In a very simple picture

the spin-splitting of the 2D states caused by the Rashba e�ect can be seen as a spin-

polarization due to the Zeemann e�ect. The e�ective magnetic �eld Beff would be ~k-

dependent and described by αR(~k|| × ~ez). The direction of Beff , i.e. the spin quantizationaxis, would be given by the vector product and the size of the splitting is determined by

the Rashba constant αR, which is proportional to the gradient of the potential con�ning

the electrons to the surface. But within the framework of the quasi-free electron model

typical values for the spin splitting would be several orders of magnitude smaller than

experimentally observed [25, 26]. Using a simple tight binding model it was shown [25]

that αR is proportional to the atomic SOC and an asymmetry parameter γ.

Recently, it was proposed by Park et al. [27] that the Rashba-type spin-splitting is a

consequence of the existence of local OAM. The local OAM is the quantum number given

10

2.2. Spin-polarized surface states

by the orbital angular momentum operator L, often called the magnetic quantum number.

The OAM produces an asymmetric charge distribution by inducing small dipoles. The

electric �eld perpendicular to the surface aligns the electric dipole and results in chiral

OAM states and the spin splitting. The characteristic chiral spin structure is formed

through SOC and is claimed to be a consequence of the chiral OAM. The authors show

that by considering the OAM as the origin of the spin splitting the predicted size of the

spin splitting is much closer to the measured value. They con�rm by them that the atomic

SOC size plays an important role.

In addition to the e�ort towards a theoretical understanding, it was found that the spin

splitting can be enhanced by corrugation of the surface potential and outward relaxation

of some atoms [28]. It is also possible to transfer the spin-polarized surface states on

a semiconducting substrate [29]. The main goal in the �eld of spintronics is to tune

the spin splitting via an external electrical �eld. The Rashba e�ect on semiconducting

substrates seems to build the basis for many di�erent electrical devices like the spin �eld

e�ect transistor of Datta and Das [30].

2.2.2 Topological insulators

The surface states in a 3D TI constitute another spin-polarized 2DES that is discussed in

this section. A TI is a material that has an energy gap in its bulk but is conducting at the

edges. In three dimensions, the bulk itself is insulating but the surfaces are metallic. There

are also 2D TIs, which have one-dimensional gapless edge states. As explained in Sec. 2.1.2

surface states exist in the energy band gap of the bulk material. There are topologically

trivial and non-trivial surface states. The non-trivial ones are called topological surface

states. Trivial surface states arise from and end in the same bulk band and they exist also

in projected bulk band gaps. Topological surface states, however, connect two di�erent

bulk bands and the corresponding band gap is a true bulk band gap. In addition, this

band gap is inverted, which means that the order of conduction and valence band in a TI

is reversed compared to the band structure of trivial materials. By connecting a TI with a

normal insulator like, for example, vacuum the topology of the band structure changes at

the interface. In order to restore the order of the bulk bands the band gap will be closed

and reopened, which results directly in metallic edge states at the surface.

In general, the surface states in a TI are Dirac-like and show conical dispersion but

in contrast to graphene the bands are spin-polarized because of the strong SOC. The

broken inversion symmetry at the surface dictates the spin-splitting of the surface states.

11

Chapter 2. Scienti�c Background

Time-reversal symmetry gives rise to the so-called spin-momentum locking; all electrons

with spin up (down) travel to the right (left) side. Accordingly, chiral spin textures are

found in momentum space with the sense of chirality reversed across the Dirac point.

Electrons in the surface states are immune to back scattering from disorder and non-

magnetic impurities, since for back scattering the electron would need to �ip also its spin.

Due to this fact, such surface states are extremely robust to disorder and they are called

'topologically protected'. An idealized band structure for a TI is shown in Fig. 2.5. The

simplest criterion to identify topologically non-trivial surface state is an odd number of

Fermi level crossings between the Brillouin zone center and the boundary. In the simple

example in Fig. 2.5, it would be just one crossing.

Fermi level

Momentum

Ener

gy

conduction band

valence band

Figure 2.5: An idealized band structure for a topological insulator. The Fermi level fallswithin the bulk band gap which is traversed by topologically-protected surface states.

A TI in 2D is also known as a quantum spin Hall insulator. This state was theoretically

predicted in 2005 [31] for graphene at low temperatures. Since the SOC in carbon atoms

is very small, the predicted gap is only of the order of some µ eV and experimentally not

observable. Subsequently, Bernevig et al. [32] claimed that there is a quantum spin Hall

state in HgCdTe quantum well structures. One year later the �rst experimental observation

of a TI was reported in that system [33]. Several materials of 2D TIs have been proposed

theoretically [31,32,34].

Theoretical predictions about topological surface states were also made for several 3D

materials [35, 36] like Bi1−xSbx and strained HgTe and α-Sn [37]. The �rst experimental

discovery of a 3D TI was reported in 2008 by Hsieh et al. [38]. For Bi1−xSbx �ve Fermi

level crossings were found.

Shortly later many theoretically predictions for simpler versions of 3D TIs were pub-

lished. For example, Bi2Te3, Sb2Te3 [39] and Bi2Se3 [40] should show a large bulk band

12

2.3. Surface states vs. 2D states

gap and a gapless surface state consisting of only one single Dirac cone at the Brillouin

zone center. Indeed, the linear dispersion relation of these surface states were subsequently

observed in ARPES experiments [40, 41]. Since then, the �eld has expanded at a rapid

pace [42�46]; many new compounds are predicted to be topologically non-trivial [47, 48]

and some already experimentally proven [5, 49,50].

One obstacle in real TIs is the high conductivity of the intrinsically doped bulk due

to unavoidable defects and vacancies formed during the growth procedure. In Bi2Se3, for

example, Se vacancies are responsible for the doping level of the bulk. The challenge in

every experiment is to distinguish between surface and volume e�ects. For transport mea-

surements in highly doped TIs, di�erentiation can be quite di�cult or even impossible.

Therefore, a TI with a large bulk band gap and the Fermi level inside the gap would be

desirable. There are di�erent approaches to solve this problem like, for example, reducing

bulk carrier density by doping [51,52]. One possibility is to mix the elements and get ma-

terials that ful�ll the requirements, like Bi2Te2Se [53�55]. Another option is to reduce the

thickness of the sample in order to increase the surface-to-volume ratio. For such nanofab-

rication three main methods are used; mechanical exfoliation [56], growing nanoplates

and nanoribbons by vapor-liquid-solid synthesis [57], and growth of TI nanostructures by

molecular beam epitaxy (MBE). The last approach allows for layer by layer growth with

large areas, high crystalline quality, and accurate thickness and chemical composition from

one to several quintuple layers (QLs) [58].

The surface states of TIs are not only of fundamental importance but have also great

potential applications. Despite disorder due to impurities they are predicted to stay metal-

lic even at T = 0 because of forbidden back scattering [59]. Due to the dissipation-less

transport the edge states of TIs are of huge interest for room temperature spin-based

electronic devices [60] and applications in quantum computation [46, 61]. In addition, the

helical surface states of TIs could provide access to novel physical phenomena like Majorana

fermions [62].

2.3 Surface states vs. 2D states

In addition to topological surface states, we investigated 2DESs of two other types. We had

a closer look at the electronic structure of surface alloys on Ag and we studied the e�ect of

impurity scattering in the band structure of graphene. All systems of interest in this work

are treated as 2D but the way they are fabricated and their resulting properties are quite

13

Chapter 2. Scienti�c Background

di�erent. Surface alloys on Ag, for example, show spin splitting due to the Rashba e�ect

and the graphene band structure is spin degenerate. Building a surface alloy on Ag shows

consequences for the �rst few atomic layers at the surface whereas graphene, being exactly

one atom thick, is a perfect 2D crystal. The electrons in graphene behave like massless

particles while the electronic states in the surface alloys show parabolic dispersions. In the

following section both systems are introduced and their basic principles and properties are

presented.

2.3.1 Surface alloys

Surface alloys on Ag(111) are known for their huge Rashba-type spin splitting in the surface

states [63, 64]. For the preparation of the surface alloys a third of a monolayer of Bi or

Sb is deposited on the clean Ag(111) surface. Every third atom in the Ag(111) surface is

replaced by an alloy atom and a long range ordered surface alloy is formed. The resulting

(√

3×√

3)R30◦ structure is shown in Fig. 2.6.

(a)

Δz

(b)

Figure 2.6: Surface alloys on Ag(111): (a) Top view and (b) side view of the (√

3×√

3)R30◦

structure formed by surface alloys. Every third silver atom (grey) is replaced by an alloy atom(red). The relaxation out of the surface plane is described by ∆z.

The band structure of the surface alloys has been extensively investigated and discussed

in literature [28,65]. The dispersion shows two spin-polarized bands with the characteristic

momentum o�set kR. The surface alloy Bi/Ag(111) shows a huge spin splitting of ER =

200meV. The spin-splitting mechanism and the origin of the huge Rashba energies is

not completely understood but it was shown that there are three important ingredients;

structural inversion symmetry, atomic SOC and the outward relaxation of the alloy atoms.

With increasing relaxation ∆z the asymmetry grows and the resulting spin splitting gets

larger [25, 28, 66]. It was theoretically shown that the orbital character of the bands is

determined by the relaxation, which varies for di�erent alloy atoms.

In addition to the orbital character, the spin structure is a�ected by the corrugation

of the surface potential. Surface alloys show not only in-plane but also out-of-plane spin

14

2.3. Surface states vs. 2D states

components [64,67]. This can be explained by an in-plane inversion asymmetry that results

in an in-plane component of the potential gradient at the surface [68].

All these extra features of the spin splitting are not included in the original Rashba

model. However, for building spintronic devices it would be very desirable to have one

combined theory describing all ingredients and features of the spin splitting mechanism. A

more detailed understanding of tuning the spin splitting would allow one to fabricate all

di�erent kinds of devices with the proper spin textures for any application.

2.3.2 Graphene

The last candidate for a 2DES in this work is the perfect 2D crystal found in the carbon

allotrope graphene. It is one single atomic plane of graphite and consists of sp2 bonded

carbon atoms arranged in a honeycomb lattice.

The theoretical description of a single layer of graphite was already presented in 1947

by P. R. Wallace [69], but it was believed for a long time that it would be very unstable

and impossible to isolate. In 2004, Novoselov and Geim succeeded in isolating a single

layer of graphene. They used the micromechanical exfoliation procedure, also known as

the 'Scotch tape technique' and transferred the graphene sheet onto a SiO2 substrate

[70]. After the successful experimental isolation of graphene the research on this material

increased rapidly. Many interesting e�ects could be shown like, for example, the anomalous

integer quantum Hall e�ect in graphene [71, 72]. Single layers of graphite were known

before, but the breakthrough was given by the fact that graphene on SiO2 shows an optical

contrast that makes it easy to di�erentiate single and double layer graphene. For their

�groundbreaking experiments regarding the two-dimensional material graphene� Novoselov

and Geim received the Nobel prize in physics in 2010.

The electrons in graphene behave like massless particles and can be described by the

Dirac equation. Due to the presence of two equivalent sublattices [see Fig. 2.7(a)], the wave

function shows 2-spinor character and determines the electronic properties. Graphene has

two π-bands that touch each other exactly at the Fermi energy at the K-points � the

six corners of the Brillouin zone [Fig. 2.7(b)] and behaves like a semi-metal. These points

are the so-called Dirac points. Close to those points, the bands disperse linearly and the

band structure has the shape of a cone [see Fig. 2.7(c)], where the band velocity is about

vF ≈ 106 m/s. The dispersion can be described by the following equation:

E(k||) = ~vFk||

15

Chapter 2. Scienti�c Background

(a) (b)

Γ K

M

K'

kx

ky

(c)

Figure 2.7: Structure of graphene: (a) two equivalent sublattices shown in red and blackresult in graphene's honeycomb lattice, (b) the corresponding hexagonal Brillouin zone withthe most important high symmetry points indicated. (c) Close to the K-point the bandstructure can be approximated by a cone.

Current research on graphene can be divided into two section. One is dealing with the

fundamental properties and interesting quantum e�ects that can be observed in graphene.

The other section is involved in pushing graphene further in the direction of applications in

electronic devices. But in this �eld, there are some major problems and questions to solve:

It is still not clear what causes the minimum conductivity of 4 e2/h in graphene [73, 74].

A possible explanation could be the charge puddles in graphene sheets that give rise to

higher scattering rate [75]. Another problem is the missing energy band gap in graphene

and the resulting low ratios between the 'on' and 'o�' state in a �eld e�ect transistor built

out of graphene [73].

Graphene production

In principle, there are three main approaches to produce graphene [9]: Pulling one single

layer from graphite, which is known as mechanical exfoliation, or growing a layer of carbon

on a substrate either via epitaxial growth or via chemical vapor deposition (CVD).

Exfoliation: To get one single layer of graphene by exfoliation, multiple peeling steps

with an adhesive tape until only one is left are required. After cleaving, the �akes are

transferred onto a SiO2 substrate where the number of layers can be determined with

an optical microscope. This method results in �akes with a lateral size of about one

millimeter [76]. Exfoliated graphene samples show very high quality and high charge

carrier mobility and are the best for proof-of-principle devices in basic research. However,

this technique is not suitable for large scale production of graphene.

16

2.3. Surface states vs. 2D states

Epitaxy: Graphene can be grown on various metallic substrates by CVD or epitaxially

on a semi-insulating substrate like silicon carbide (SiC) by high temperature annealing.

Already decades before the discovery of graphene in 2004, it was known that hydrocarbons

can be cracked on catalytic metal surfaces. In particular, it was shown that CVD-graphene

grows well on Ni [77�79], Rh [80], Ru [80], Ir [81,82] and Pt [80,83,84]. The advantage of

that method is the self-limiting character which leads exactly to one layer of carbon atoms.

However for many applications the metallic substrate is undesirable.

A more promising way to build graphene devices on a large scale is the epitaxial growth

on SiC wafers. Silicon has a higher vapor pressure and leaves the carbon atoms at the

surface. By heating a SiC wafer to temperatures above 1100◦C in ultra high vacuum (UHV)

graphene is formed on the surface [85]. Its thickness, electron mobility and charge carrier

density depends very much on which side of the SiC wafer is used for graphene formation.

The growth on SiC(0001̄) � the carbon-terminated or C-face � results in rotationally

disordered multilayer graphene due to the weak interaction between the graphene layers

and the substrate. Due to this rotational disorder the layers are electronically decoupled

and show pretty high carrier mobilities that are comparable with isolated graphene sheets

[86,87]. However, controlling the thickness is quite limited on that side [88,89].

On the opposite side � the silicon-terminated or Si-face � graphene grows in large

sheet and covers whole terraces [89�92]. However, the commercially available SiC wafers

have typically a lot of scratches on this surface, which have to be removed by hydrogen

etching at elevated temperatures. After etching away several hundred nanometers the

surface show large and clean terraces with a width of 1500Å and a step height of only one

unit cell [93,94]. The following annealing step can either take place in UHV or in 900mbar

Ar. Graphitization of SiC in UHV is accompanied by a considerable roughening of the

surface. This can be avoided by annealing in Ar at elevated temperatures, which results in

step bunching and much larger terraces [95]. In both cases, the �rst carbon layer that is

formed has a honeycomb structure, but does not show graphene-like electronic properties.

Since every third atom of the carbon layer is sp3 hybridized and covalently bound to the

substrate the π-bands cannot be formed [96]. The growth process is schematically drawn

in Fig. 2.8.

In addition, this so-called zerolayer forms a (6√

3 × 6√

3)R30◦ reconstruction with

respect to the SiC substrate [88, 91, 98�100]. With increasing temperature further carbon

layers will be formed. The second carbon layer is called monolayer graphene [see Fig.

2.8 (b)] and shows a Dirac cone at the K-point. However, the band structure contains

17

Chapter 2. Scienti�c Background

Figure 2.8: Side view models for (a) the (6√

3 × 6√

3)R30◦ reconstruction of SiC(0001)(called zerolayer) and (b) epitaxial monolayer graphene (taken from [97]).

signatures of the substrate. Due to charge transfer from the substrate to the graphene layer

the Dirac point is about 420meV below the Fermi level [97,101�103] and the charge carrier

mobility is quite low compared to exfoliated graphene [104]. Since nucleation of a new

graphene layer starts at step edges, Ar-annealed samples are much more homogeneously

covered [95]. By choosing the right annealing temperature and duration the number of

graphene layers can be controlled quite easily.

18

Chapter 3

Experimental Techniques

3.1 Photoemission spectroscopy

Photoemission spectroscopy (PES) is based on the photoelectric e�ect discovered by H.

Hertz in 1887 [105]. About 20 years later Einstein was able to explain this e�ect by

postulating the quantum nature of light [106], for which he was awarded the Nobel prize in

physics in 1921. In the following sections an introduction to this experimental technique

and a theoretical description are given.

3.1.1 The photoemission process

Light exists as discrete quantized packets called photons, with an energy ~ω. If theyimpinge on a surface and their energy is larger than a characteristic value Φ, called the

work function, they release electrons with kinetic energy Ekin from the surface. If Ekin is

measured by an analyzer, the binding energy EB of the electron can be determined via

EB = ~ω − Φ− Ekin (3.1)

For photoemission measurements the work function of the spectrometer has to be used.

Sample and spectrometer are usually in electrical contact and thus the Fermi level is

aligned. All relevant energies involved in the photoemission process are shown in Fig. 3.1.

Note that EB is referenced to the Fermi level (EF is equivalent to zero binding energy),

while the kinetic energy is measured with respect to the vacuum level. Depending on

the energy of the incident photons there are two di�erent types of photoemission spec-

troscopy experiments: For the excitation of valence electrons, photons in the ultraviolet

19

Chapter 3. Experimental Techniques

Evac

EF

N(E)

EvacEF

EB

core levels

valence band

ΦS ΦA N(E)

hν

hν

PES spectrumEkin

sample

Figure 3.1: Schematic illustration of the energies involved in a photoelectron emission pro-cess from a solid. N(E) is the energy distribution of the photoemitted electrons. After [107].

(UV) range are used (ultraviolet photoemission spectroscopy, UPS) whereas the use of

x-rays gives access to the core levels, electronic states with much higher binding energy

(x-ray photoemission spectroscopy, XPS).

Since Eq. 3.1 is only valid for electrons that did not experience any inelastic event

while leaving the material, the probing depth of those techniques can be estimated by the

mean free path λ of the electrons which gives the average distance electrons travel without

energy loss. It is a measure for the escape depth of the electrons in a solid. For the relevant

energies in PES the electrons can be described as a free electron gas. In this case λ depends

only on the electron concentration. Since this is roughly equal in all materials the mean

free path follows a universal curve that is shown in Fig. 3.2. This curve can be described

20

3.1. Photoemission spectroscopy

1

2

4

6

10

2

4

6

100

mea

n fr

ee p

ath

(Å)

100

101

102

103

104

energy (eV)

Figure 3.2: Universal curve: Mean free path as function of energy, calculated using Eq. 3.2.The escape depth of the electrons in a solid is almost independent of the material. For therelevant energies the mean free path is about several Å.

by the phenomenological function [108]

λ(E) =538

E2+ 0.41

√aE (3.2)

where a is the thickness of a monolayer in nm. The curve has a broad minimum in the

energy range of 50-100 eV. Using those energies for PES means that the escaping electrons

originate from the �rst few atomic layers at the surface. This makes PES a very surface

sensitive technique.

The photoemission of an electron [Eq. 3.1] can be described in a simple picture as

follows: A photon impinges on a surface of a solid and excites an electron via the photo-

electric e�ect. The excited electron escapes into the vacuum while energy and momentum

have to be conserved. Since the photon momentum is small compared to the momentum

of the electron ~k, it can be neglected. The resulting direct transition is possible in a crystal

lattice, where a lattice vector can compensate for the missing momentum [compare Sec.

2.1.1]. For a quantitative interpretation of photoemission experiments a more elaborate

picture of the photoemission process is needed.

There are two basic approaches to describe the photoemission process theoretically:

The rather simple three-step model and the more realistic one-step model. The following

theoretical description is based on the references [9, 107, 109]. Within the framework of

the three-step model the process is decomposed into three independent steps; (1) electron

21

Chapter 3. Experimental Techniques

excitation, (2) electron propagation to the surface and (3) escape through the surface

into vacuum [see Fig. 3.3]. Here it has to be pointed out that only elastically scattered

electrons are of interest since only those carry information about the initial state in the

solid. The measured photocurrent I is proportional to the product of the probability of the

photoexcitation, the probability of the electron traveling to the crystal-vacuum interface

without being scattered, and the transmission function for the interface.

The separation into three independent steps is somewhat arti�cial. In the so-called

one-step model this is eliminated and the whole photoemission process is considered as one

single step. It describes the excitation from an initial Bloch state into a damped �nal state

near the surface. This damping takes care of the short mean free path of the electrons in

a solid.

E

Ef

Ei

0z

excitation

propagation escape

1

2 3

Figure 3.3: Schematic drawing of the three-step model. The photoemission process is dividedinto three steps; (1) photoexcitation, (2) electron propagation to the surface and (3) escapethrough the surface into vacuum.

The calculation of the photocurrent is based on Fermi's Golden Rule. For making the

calculation feasible the sudden approximation [107] is mostly used. Here, the electron

is assumed to immediately exit the surface of the material, without interacting with the

remaining electrons and the photohole it leaves behind. The photocurrent is then propor-

tional to the transition probability ωfi from the initial Ψi to the �nal state Ψf . Using the

dipole approximation gives [107]

I ∝ 2π~|〈Ψf | ~A~p|Ψi〉|2δ(Ef − Ei − ~ω)

22

3.1. Photoemission spectroscopy

To simplify the transition matrix element a one-electron view is taken for the initial

and �nal state wave function. The initial state can be written as a product of the orbital

Φi,~k from which the electron is excited, and the wave function of the remaining electrons:

ΨNi = Φi,kΨki (N − 1)

Accordingly, the �nal state is written as a product of the wave function of the pho-

toemitted electron Φf,Ekin and that of the remaining (N − 1) electrons:

ΨNf = Φf,EkinΨkf (N − 1)

The square of the absolute value of the wave function of the remaining electrons gives

the spectral function, i.e.∑|〈Ψkf (N − 1)|Ψki (N − 1)〉|2 = A(~k,E), and the photocurrent

turns into

I ∝∑f,i,~k

|〈Φf,Ekin|~r|Φi,k〉|2A(~k,E)f(E, T )

where f(E, T ) = (eβ(E−µ)+1)−1 is the Fermi-Dirac distribution function that accounts

for the occupation of the electronic states with β = (kBT )−1, the Boltzmann constant kBand the chemical potential µ. The spectral function can be related to the single particle

Green's function G(~k, E) via

A(~k,E) =1

πIm(G(~k, E)

)The Green's function for a system with non-interacting electrons is given by the formula

G0(~k,E) = 1/(E − E0~k − iγ), where γ is a in�nitesimally small number and E0~kis the

dispersion E0~k = ~2~k2/(2m∗). The corresponding spectral function in this case is a δ-

function A0(~k, E) = 1πδ(E − E0~k).

3.1.2 Quasiparticle picture

So far, all formulas were based on the independent electron approximation, which cov-

ers a single electron moving in an e�ective potential Ueff (~r) of the atomic cores and the

remaining (N − 1) electrons with the resulting bare band dispersion E0~k . For a completedescription of an electron in a solid, one has to account also for many-body e�ects, resulting

in the independent electron picture breaking down. However, the properties of a system

with interacting electrons, called a 'Fermi liquid', can be mapped onto those of a system

23

Chapter 3. Experimental Techniques

of non-interacting electrons by a formalism of Landau. The bare electron combined with

many-body interactions are handled as new particles, so-called 'quasi-particle'. The main

conclusions of the independent electron approximation remain valid. The spectral proper-

ties measured by photoemission spectroscopy of a Fermi liquid di�er in four respects from

the free electron gas [107]: (1) The energy of the interacting system (E~k) is renormalized

relative to that of the non-interacting system (E0~k). (2) The quasi-particles have a �nite

lifetime. (3) There is an incoherent background due to electron-hole pairs. (4) The height

of the Fermi step is reduced.

In systems where many-body interactions are taken into account, it is useful to introduce

the so-called self-energy Σ(~k,E), which accounts for the renormalization of the electron

energy. The Green's function turns into G(~k, E) = 1E−E0

~k−Σ(~k,E)

and the spectral function

for an interacting system is given by

A(~k,E) =1

π

Im(

Σ(~k, E))

[E − E0~k −Re

(Σ(~k,E)

)]2+[Im(

Σ(~k,E))]2 (3.3)

In the simplest case, Im(Σ) is constant and Re(Σ) = 0. The spectral function is then

a Lorentzian at E0~k with full width at half maximum Γ = 2Im(Σ). The real part of Σ

causes deviations from the bare energy dispersion E0~k and the imaginary part is responsible

for the linewidth. The latter includes the intrinsic linewidth as well as broadening due to

interactions. E0~k is solely determined by the symmetries of the lattice potential. All the

in�uences of many-body interactions like electron-electron and electron-phonon scattering

can be expressed in terms of the complex self-energy Σ.

With ARPES one yields information about the properties of the quasi-particles, i.e.

one measures the renormalized dispersion. Due to the high resolution of state-of-the-art

analyzers a very accurate determination of the photoemission linewidth is possible and

ARPES became a powerful tool for the investigation of many-body interactions in solids.

For two- or one-dimensional electronic states the measured linewidth corresponds to the

width of the hole state and equals the imaginary part of the self-energy. In this case

the full-width-at-half-maximum (FWHM) of the photoemission peaks is related to the

quasiparticle lifetime τ via τ = ~/Γ. The quasiparticle lifetime is a sum of three maincontributions

Γ = Γe−e + Γe−ph + Γe−imp

where Γe−e is the electron-electron scattering, Γe−ph the electron-phonon scattering and

24

3.2. Angular resolved photoemission

Γe−imp the impurity scattering [110].

For an electron at the Fermi level, Γe−e = 0 when T = 0, which means there is no phase

space for any scattering events and the lifetime of the electron is in�nite. At energies

E < EF , the scattering rate is proportional to (E −EF )2. At �nite temperature there willbe partially occupied electronic levels in a shell of width kBT about EF . The scattering

rate is then proportional to (kBT )2. The total scattering rate due to electron-electron

interaction is therefore

Γe−e = 2β[(πkBT )2 + (E − EF )2] (3.4)

with the electron-electron interaction constant β. In the case of electron-phonon scat-

tering not only the lifetime is a�ected but also the energy dispersion. The band renormal-

ization due to electron-phonon scattering can be expressed as a change of the electronic

velocity v(k) = 1/~(∂E/∂k). The renormalized velocity can be calculated via [111]

v(k) =1

1 + λv0(k)

with the velocity of the non-interacting case v0(k) = 1/~(∂E0/∂k) and the electron-phononcoupling constant λ. Electron-phonon interactions decrease the slope of the dispersing

bands and lead to a kink around the Fermi level. The contribution to the linewidth due

to scattering at impurities is independent of energy E and temperature T . It is a constant

contribution (Γe−imp = const.) and changes only with impurity concentration.

3.2 Angular resolved photoemission

With an angular resolved photoemission experiment it is possible to determine the angular

dependence of photoemitted valence band electrons as a function of their binding energy.

Therefore, not only the kinetic energy Ekin, but also the emission angle θ of the photoelec-

tron is measured. When the photoexcited electron passes through the surface into vacuum

a free-electron like �nal state with Ekin = p2/2m is assumed. While escaping, the electron

momentum perpendicular to the surface is changed but the in-plane component k|| is con-

served. According to Fig. 3.4 k|| can be determined directly from the emission angle θ of

the photoelectron via

k|| [Å−1] =

√2meEkin

~2sin(θ) = 0.512

√Ekin [eV] sin(θ)

25

Chapter 3. Experimental Techniques

where me is the electron mass and θ the angle between k|| and normal emission. The

binding energy of the electron in the initial state is determined as before using Eq. 3.1.

vacuum

crystalθi

θ

z

k||,int

k||,ext

k ,intkint

k ,ext p/h

k||,int =k||,ext =p/h

Figure 3.4: Relations between the crystal momentum and the measured electron momentumin the free-electron �nal state approximation.

The setup for an angular resolved photoemission spectroscopy (ARPES) experiment

consists of a photon source in the UV range and an electrostatic analyzer that measures

Ekin and θ. The photon source can either be a gas discharge lamp, a laser or synchrotron

radiation. The typical beam spot size of a UV source is 1mm2, whereas at the synchrotron

the illuminated area can be much smaller and the intensity much higher. Concerning the

analyzer, the availability of 2D charge-coupled device (CCD) detectors has made ARPES

an extremely detailed and precise tool to directly measure the electronic band structure

(EB(k||)) of a 2DES. A typical setup is shown in Fig. 3.5. The in-plane momentum can be

varied by turning the sample around θ and Φ, respectively, as indicated.

For the analysis of photoemission data the 2D spectra are usually divided into ei-

ther momentum distribution curves (MDCs) or energy distribution curves (EDCs). While

MDCs show the photocurrent as a function of the emission angle at a constant binding

energy, EDCs display the measured intensity at a constant emission angle dependent on

the binding energy. For quantitative conclusions an appropriate background has to be

subtracted from the spectra. Therefore, the spectrum is divided into a primary spectrum

and a secondary spectrum where the latter represents inelastic events like electron-electron

and electron-ion scattering [107]. There are several sophisticated formulas for backgrounds,

like for example the version given by Tougaard [112], but usually it is su�cient to apply

a constant background that accounts for the dark count rate in the detector plus the so-

called Shirley background BS(E). This type of background is proportional to the weight

26

3.2. Angular resolved photoemission

UV photonshν

phot

oele

ctro

ns

hemispherical analyzer

2D detector

sample

Φ

θ

Figure 3.5: Typical angular resolved photoemission setup: Photons with the energy hν im-pinge on the sample surface and excite electrons. The emitted photoelectrons are focused intoa hemispherical analyzer. The kinetic energy as well as the emission angle will be measured.The emission angle is varied by turning the sample around θ and Φ and the third direction iscovered by the acceptance angle of the analyzer. After passing the analyzer the electrons aredetected with a 2D CCD camera.

27

Chapter 3. Experimental Techniques

of the primary spectrum [107]. When analyzing EDCs one has to consider also the cut-o�

at the Fermi level due to the change in occupation of the electronic states. For the �tting

procedure of the remaining primary spectrum peaks with a Voigt line shape, a convolution

of Lorentzian and Gaussian functions, are used. The complete �tting function for an EDC

is given by:

I(E) = c+BS(E) +

[∑i

L(E,Ei,Γi) ∗G(Γres)

]f(E − EF , T )

The constant o�set c accounts for the dark count rate in the detector. L(E,Ei,Γi) are the

Lorentzians [see Eq. 3.3] with the peak positions at Ei and the full width at half maximum

Γi = 2Im(Σ) that describe the single peaks. The Gaussian function G(Γres) accounts for

the experimental resolution Γres.

The measurements presented in Chap. 4 and 5 have been carried out at the Max

Planck Institute for Solid State Research (MPI-FKF) in Stuttgart. A hemispherical SPECS

electron analyzer (energy and angular resolution are 15meV and 0.5◦, respectively) and

a monochromatized He lamp that o�ers UV radiation at hν = 21.2 eV (He I) and hν =

40.8 eV (He II) are attached to the UHV chamber with a base pressure p = 2 · 10−10 mbar.The manipulator can be cooled with liquid nitrogen to about −180 ◦C.

The ARPES experiments shown in Chap. 6 have been performed at the University of

British Columbia in Vancouver. The UHV chamber is equipped with a SPECS Phoibos

150 hemispherical analyzer and a UVS300 monochromatized gas discharge lamp. Energy

and angular resolution were set to 15meV and 0.3◦. Linearly polarized photons with an

energy of 40.8 eV were used. During ARPES measurements the samples were kept at 8K

at a pressure less than 7 · 10−11 mbar.

The data shown in Chap. 7 were taken at the Synchrotron Radiation Center (SRC)

in Stoughton, Wisconsin, USA at the variable polarization VLS-PGM beamline. This

beamline was equipped with an elliptically polarized Apple II undulator that delivers p-

and s-polarization of photons in an energy range from 15 eV to 250 eV. A Scienta analyzer

with an energy resolution of about 10meV and an angular resolution of 0.4◦ has been used.

The manipulator could be cooled with liquid helium down to 30K. The base pressure of

the UHV chamber was p = 1 · 10−10 mbar.

28

3.3. Core level spectroscopy

3.3 Core level spectroscopy

Core level spectroscopy, also known as X-ray photoemission spectroscopy (XPS) is a pow-

erful tool to study the chemical composition or to determine the binding energies of the

atomic core levels of elements in a solid [113]. A photon source that delivers photons in the

soft X-ray region is needed to provide enough energy for excitation of core electrons. The

binding energy of the core levels is determined by measuring Ekin of the photoelectrons for

normal emission and using Eq. 3.1. A schematic illustration of the photoemission process

in XPS is drawn in Fig. 3.1.

Since every element has a characteristic series of binding energies for its core electrons

XPS serves to determine the chemical composition of the sample surface by comparing the

measured peak positions to reference spectra. For precise identi�cation one can additionally

check the intensity ratio and separation of some spin doublets for p, d and f lines. Due

to SOC all core levels with non-zero angular momentum (l 6= 0) are split into branches.Furthermore the holes created in the atoms give rise to the emission of so-called Auger

electrons, which can be detected in the spectrum too.

When elements are mixed in compounds, the binding energy of the peak under inves-

tigation shifts slightly by an amount ∆EB, which is called the chemical shift. Whether

this shift is positive or negative is determined by the e�ective electronic potential variation

induced by the charge distribution between the elements forming the compound. Further-

more, the shift depends on the bonding type, on the electronegativity of the elements, and

on the interaction between the photoionized atom and the rest of the crystal [107]. By

measuring the small shifts one can use XPS to determine the chemical state of an atom.

This is the reason why formerly XPS was also called ESCA which stands for electron

spectroscopy for chemical analysis.

It is also possible to analyze XPS spectra quantitatively. The integrated intensity of

the peaks give access to the concentration of a particular material. One has to take care

about the secondary electrons. The main peaks in the photoemission spectrum correspond

to electrons that leave the surface without energy loss. Electrons that undergo inelastic

scattering events contribute to the Shirley background.

All core level spectra shown in this thesis were measured at the MPI-FKF in Stuttgart.

The measurements have been performed at room temperature using non-monochromatized

Mg Kα radiation at hν = 1253.6 eV. The spot size of a conventional X-ray source is about

a few mm2. XPS has been used mainly to check the cleanliness of the substrate.

29

Chapter 3. Experimental Techniques

30

Chapter 4

Coulomb interaction in topological

insulators

A 3D TI is a quantum state of matter characterized by an insulating bulk state and gapless

surface states that show a peculiar spin texture [see Sec. 2.2.2]. Possible applications of TIs

in electronic devices require a highly insulating bulk and tunable Dirac carriers. Due to the

coexistence of both bulk and surface conduction in Bi2Se3, it is di�cult to investigate the

topological properties separately. In ongoing research, there are extensive e�orts to reduce

bulk carriers in Bi2Se3 through material doping [41,51,114], nanostructuring [57,115,116]

and electric gating [117,118]. By replacing Se with Te atoms, the bulk insulating property

could be considerably improved. Accordingly, Bi2Te2Se is a system where the energy gap

is ∆ ≈ 0.3 eV and the chemical potential is located within the bulk band gap [119].

Common theoretical descriptions of TIs are formulated in terms of single-particle quan-

tum mechanics. Due to quite large lattice dielectric constants (> 50) in TIs and the very

small corresponding e�ective �ne structure constant, it is often claimed that electron-

electron interactions are negligible and does not alter the topological properties [59]. But

it was shown that the electron-electron interaction is often needed to describe experimental

observations [120�122]. If the interaction is very strong it can even turn the topological

phase into an insulating ground state [6] or induce a novel critical state on the surface [123].

Therefore, it is a crucial issue to understand the interplay between strong electron-electron

interaction and the topological surface states [124,125].

31

Chapter 4. Coulomb interaction in topological insulators

4.1 Bi2Se3, Bi2Te3 and Bi2Te2Se

The 3D TIs Bi2Se3 and Bi2Te3 and also the mixture Bi2Te2Se have a tetradymite structure.

All materials of this family crystallize in covalently bonded QLs weakly interacting via van

der Waals force [5]. As shown in Fig. 4.1(a) the stacking order is A-B-C-A-B-C. Each

quintuple layer is about 1 nm thick and the lattice constant along the c-axis is about 3 nm.

TeBiSeBiTe

BiTeSe

(a)

unit

cell

(b)

Figure 4.1: Crystal structure of tetradymite chalcogenides, using the example of Bi2Te2Seand the corresponding surface band structure. (a) QL enclosed by the brown cage is thebuilding block of this type of materials. The stacking order of the QLs is A-B-C-A-B-C, andhence the unit cell consists of a stack of 3 QLs. (b) Topological surface state measured withARPES.

The interesting properties of those materials are connected to their electronic structure

and, particularly, the low energy region. The states close to the Fermi energy are mainly p

orbitals. Therefore, the opposite parities originate from bonding and anti-bonding states.

By taking into account chemical bonding, crystal �eld splitting and SOC, a pair of inverted

energy bands is found at the Fermi level. This inversion drives the system into a TI

phase. The bulk insulating gap is ∆ ≈ 0.3 eV, which results in the possibility of havinga topological phase at room temperature. To describe the low-energy properties of those

systems an e�ective Dirac model is used.

Due to naturally occurring crystalline defects in Bi2Se3 and Bi2Te3, their bulk is always

highly doped and their transport properties are always dominated by bulk carriers. The

32

4.2. Doping behavior

key for the preparation of a TI with large bulk resistivity is to shift the Fermi level into

the bulk band gap. For example, by mixing Te and Se atoms, Bi2Te2Se can be fabricated,

in which the chemical potential is located between valence and conduction band of the

bulk and which shows a large bulk resistivity exceeding 1Ωcm [119]. By this shift of the

chemical potential the contribution from the surface states to the conducting electrons is

strongly enhanced. It is the �rst 3D TI where detailed transport studies of the topological

surface state are possible. Clear Shubnikov-de Haas oscillations are observed and they

contribute ∼ 6% to the total conductance in a 260-µm-thick bulk crystal. Xiong andcoworkers reported an even larger resistivity of 6Ωcm [126].

For the investigation of the surface state band structure including many-body e�ects in

3D TIs ARPES is the technique of choice. ARPES probes directly the 2D band structure

which contains all the many-body phenomena [see Chap. 3.1.2]. Bi2Te2Se crystals were

grown in the group of Prof. Claudia Felser at the MPI-CPfS in Dresden. The samples were

glued to a sample holder and cleaved in vacuum via mechanical exfoliation. As a photon

source, the HeI line was used. In Fig. 4.1(b) the band structure of a freshly cleaved surface

is presented. This measurement and all subsequent ones on this system were performed at

room temperature. The topological surface state in the bulk band gap is clearly visible. The

Dirac point almost coincides with the top of the valence band at around EB = 0.2 eV. From

the Fermi level down to this point we only see the Dirac cone and a very low background.

There are only the topological states at the Fermi level and for them back scattering is

forbidden. Hence, the bands are quite sharp and they are almost linear dispersing. We

note that there is no sign of the conduction band visible at the Fermi level and that the

resulting bulk band gap is quite big. All our experimental �ndings coincide with previous

ARPES measurements [55].

4.2 Doping behavior

If the freshly cleaved sample is left in the UHV chamber for some time, a shift of the Dirac

point to higher binding energies can be observed. This time-dependent doping e�ect can

be explained by contamination of the surface from residual gas in UHV. The adsorbates

give rise to a strong band bending of the bands near the surface. A similar e�ect was also

observed for Bi2Se3 [127, 128]. In Fig. 4.2 the band structure measured at di�erent delay

times with respect to the cleavage procedure is shown.

The small black arrows indicate the position of the Dirac point, which shifts to higher

33

Chapter 4. Coulomb interaction in topological insulators

-0.1 0 0.1

k (Å-1

)

-0.1 0 0.1

k (Å-1

)

-0.1 0 0.1

k (Å-1

)

-0.8

-0.6

-0.4

-0.2

0.0

0.2In

itial

Sta

te E

nerg

y (e

V)

-0.1 0 0.1

k (Å-1

)

0 h 25 h18 h1 h

Figure 4.2: Time-dependent doping of the topological surface state at Γ in Bi2Te2Se whileresting in vacuum. Dirac point shifts to higher binding energy over time as indicated by theblack arrows. The duration between cleave and measurement is indicated in the upper rightcorner of the panels.

binding energy over time. After 25 hours the total shift of the Dirac point amounts 170meV.

Despite the large shift, we still do not see any indication from the conduction band at the

Fermi level. Hence, we conclude that the gap is at least ∆ = 0.37 eV. Due to the band

bending, the charge carrier density n increases. We determined the Fermi wave vector kFand extracted n. Both are graphically shown in Fig. 4.3.

Both kF and the corresponding n increase over time. Since we have only four data

points we can just surmise that in the beginning the band bending goes almost linearly

whereas it starts to saturate after 18 hours. During roughly one day in UHV the charge

carrier density increases by the factor of 2.8 due to adsorption of residual gas molecules.

This gives us the opportunity to study the e�ect of di�erent charge carrier densities on the

strength of many-body interactions in TIs.

4.3 Coulomb interaction at low charge carrier densities

The images in Fig. 4.2 show clearly the shift of the surface states to higher binding energies

(as indicated by the small arrows) and the increase of the Fermi wave vector kF over time.

To evaluate the many-body physics in the system we had a closer look at the linewidth,

since it is proportional to the imaginary part of the self-energy. In the following analysis

we stick to the extreme cases - the freshly cleaved, clean sample and the one that remained

for 25 hours in vacuum (now called the 'aged sample'). We took the single MDCs and

34

4.3. Coulomb interaction at low charge carrier densities

0.12

0.11

0.10

0.09

0.08

0.07

0.06

Ferm

i wav

e ve

ctor

(Å

-1)

2520151050hours after cleave

14

12

10

8

6

4

2

0

charge carrier density (1012cm

-2)

Figure 4.3: Time-dependent increase of the Fermi wave vector kF as well as the chargecarrier density n in Bi2Te2Se.

�tted them as exemplarily shown in Fig. 4.4(a). Presumably, an imperfect alignment

of the sample leads to a di�erence in linewidth of the left and the right branch and we

determined them separately. The extracted linewidth from every single peak of the left

branch as a function of binding energy for the clean and the aged sample is plotted in Fig.

4.4(b).

For both the clean and the aged sample the linewidth has a minimal value at the Fermi

level and increases with increasing binding energy. We also notice that the absolute value

of the linewidth at the Fermi level is larger for the aged sample. This can be explained

by the adsorbed gas molecules, which induce disorder at the surface leading to a constant

o�set in the linewidth. In fact, the linewidth for the aged sample is larger at the Fermi

level, but the increase of the linewidth is smaller.

As introduced in Sec. 3.1.2 there are two energy dependent scattering mechanisms

that can contribute to broadening of the linewidth; electron-electron and electron-phonon

interaction. The Debye temperature TD in Bi2Te2Se is assumed to be comparable to the

one in Bi2Se3, which is TD = 182K (∼ 16meV) [129]. Since our measurements wereperformed at room temperature the thermal energy is above TD and we do not expect

an energy dependent contribution due to interaction with phonons. Therefore, we instead

attribute the energy dependent increase of the linewidth to electron-electron interactions.

The di�erence in the increase of the linewidth can be explained by varying screening

35

Chapter 4. Coulomb interaction in topological insulators

Inte

nsity

(ar

b. u

nits

)

-0.10 0.00 0.10

Momentum (Å-1

)

(a) (b)

0.04

0.03

0.02

linew

idth

(Å

-1)

-0.10 0.00E-EF (eV)

aged clean

left branch

Figure 4.4: (a) Exemplary �t of two Lorentzian to a MDC cut through the topologicalsurface state. (b) Increase of the linewidth as a function of energy for two di�erent dopinglevels.

strength due to the di�erence in the total number of charge carriers. The only di�erence

between the two samples is the charge carrier concentration at the Fermi level. Due to

doping, i.e. the shift to higher binding energies, and the linear dispersion the Fermi surface

volume increases over time, which results in a higher charge carrier density at zero binding

energy. The more electrons are available, the higher the screening of the interaction. If

the interaction is e�ciently screened the linewidth broadening due to electron-electron

interactions is reduced.

In addition to the change in linewidth, we observe a change of the Fermi velocity, i.e.

the slope of the bands at the Fermi level, over time [see Fig. 4.5]. We noticed that the

band velocity at the Fermi level is bigger for the aged sample. This can be explained by a

renormalization of the Fermi velocity due to the electron-electron interaction, which results

in a band that disperses less steep compared to the non-interacting case. Since the number

of charge carriers increases by going from the clean to the aged sample, the e�ciency of

the screening rises and hence, the band velocity increases over time.

For more quantitative statements about linewidth and band velocity, we compare the

results of the MDC �ts to a theoretical model. With data sets at di�erent doping levels and

by considering self-consistency we are able to determine the parameters for the complex

self-energy and the bare band dispersion. We performed model calculations in 2D for the

36

4.3. Coulomb interaction at low charge carrier densities

-0.12

-0.08

-0.04

0.00

E-E

F (

eV)

-0.10 -0.05 0.00 0.05 0.10

Momentum (Å-1

)

bare dispersion 0h 25h

(shifted by 0.175eV)

Figure 4.5: Comparison of the band dispersion close to the Fermi energy. To be able tocompare the slopes, the band structure of the aged sample was shifted by 0.175 eV to smallerbinding energies. For the freshly cleaved sample we observe the smallest slope, since screeningis not su�cient due to the small number of charge carriers.

spectral function [see Eq. 3.3] by assuming a bare band dispersion of the form

E0~k = vF |~k|+ �0 (4.1)

Since we attribute the increase of the linewidth and the Fermi velocity to electron-

electron interactions we assume a quadratic energy dependence (ImΣ(ω) ∝ ω2, see Eq.3.4) for the imaginary part of the self-energy [130]. The imaginary and the real part of

the complex self-energy are connected via a Hilbert transformation H: ReΣ = H(ImΣ).Therefore, we choose for the self-energy the following ansatz:

Σ(ω) = i(β1ω2 + α)− β2ω (4.2)

The parameter α serves as a constant o�set in the linewidth, while β1 forms the real

part and β2 is the coupling constant for electron-electron interaction. For reasons of self-

consistency, the ratio between the coe�cients will be held constant β1/β2 = const. for

all doping levels. In our case the ratio was fou